LMucko/crystallography-open-database huggingface dataset:
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121257
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.6551(46)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.43283(45)
_cell_length_b                   5.40633(65)
_cell_length_c                   11.91039(84)
_cell_measurement_temperature    20
_cell_volume                     333.35(5)
_diffrn_ambient_temperature      20
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_2.cif
_cod_data_source_block           LiTCNE-20K
_cod_original_cell_volume        333.351(76)
_cod_database_code               4121257
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121258
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5467(44)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.43311(50)
_cell_length_b                   5.40704(62)
_cell_length_c                   11.91853(83)
_cell_measurement_temperature    50
_cell_volume                     333.84(5)
_diffrn_ambient_temperature      50
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_3.cif
_cod_data_source_block           LiTCNE-50K
_cod_original_cell_volume        333.840(79)
_cod_database_code               4121258
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121259
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.2844(65)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.42900(44)
_cell_length_b                   5.40499(76)
_cell_length_c                   11.9282(10)
_cell_measurement_temperature    100
_cell_volume                     334.21(6)
_diffrn_ambient_temperature      100
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_4.cif
_cod_data_source_block           LiTCNE-100K
_cod_original_cell_volume        334.212(85)
_cod_database_code               4121259
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121260
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.9947(64)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.42859(53)
_cell_length_b                   5.40755(57)
_cell_length_c                   11.94771(70)
_cell_measurement_temperature    150
_cell_volume                     335.41(5)
_diffrn_ambient_temperature      150
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_5.cif
_cod_data_source_block           LiTCNE-150K
_cod_original_cell_volume        335.413(73)
_cod_database_code               4121260
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121261
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.6921(41)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.42943(33)
_cell_length_b                   5.41232(88)
_cell_length_c                   11.9671(18)
_cell_measurement_temperature    200
_cell_volume                     336.84(8)
_diffrn_ambient_temperature      200
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_6.cif
_cod_data_source_block           LiTCNE-200K
_cod_original_cell_volume        336.84(11)
_cod_database_code               4121261
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121262
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.3790(75)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.42769(52)
_cell_length_b                   5.41077(57)
_cell_length_c                   11.9807(10)
_cell_measurement_temperature    250
_cell_volume                     337.57(6)
_diffrn_ambient_temperature      250
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_7.cif
_cod_data_source_block           LiTCNE-250K
_cod_original_cell_volume        337.570(82)
_cod_database_code               4121262
Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE = Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid Structure
Jae-Hyuk Her; Peter W. Stephens; Royce A. Davidson; Kil Sik Min; Joshua D. Bagnato; Kipp van Schooten; Christoph Boehme; Joel S. Miller; Journal of the American Chemical Society 135 (2013) 18060–18063; doi:10.1021/ja410818e

data_4121263
_publ_section_title
;
 Weak Ferromagnetic Ordering of the Li+[TCNE].- (TCNE =
 Tetracyanoethylene) Organic Magnet with an Interpenetrating Diamondoid
 Structure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18060
_journal_page_last               18063
_journal_paper_doi               10.1021/ja410818e
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C6 Li N4'
_chemical_formula_weight         135.04
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.0671(41)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.42719(39)
_cell_length_b                   5.41329(45)
_cell_length_c                   12.0020(11)
_cell_measurement_temperature    295
_cell_volume                     338.83(5)
_diffrn_ambient_temperature      295
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'double Si(111)'
_diffrn_radiation_wavelength     0.690779
_diffrn_source                   synchrotron
_exptl_absorpt_correction_type   none
_pd_char_colour                  'dark green yellow'
_pd_instr_location
; 
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        40
_pd_meas_2theta_range_min        4
_pd_meas_number_of_points        7201
_pd_meas_scan_method             step
_pd_spec_mounting
;
Sealed glass capillary of 1 mm nom diameter
;
_pd_spec_mount_mode              reflection
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_cod_data_source_file            ja410818e_si_001_8.cif
_cod_data_source_block           LiTCNE-295Ka
_cod_original_cell_volume        338.832(56)
_cod_database_code               4121263
On two new K~2~FeF~5~ forms
Le Bail, Armel; Powder Diffraction 29 (2014) 33–41; doi:10.1017/S0885715613001334

data_1513881
_publ_contact_author_address
; 
Universit\'e du Maine, Institut des Mol\'ecules et des Mat\'eriaux du Mans, 
CNRS UMR 6283, 72085 Le Mans, France
;
_publ_contact_author_email       armel.le_bail@univ-lemans.fr
_publ_contact_author_fax         '33 (0)2 43 83 35 06'
_publ_contact_author_name        'Armel Le Bail'
_publ_contact_author_phone       '33 (0)2 43 83 33 47'
_publ_section_title
;
 On two new K~2~FeF~5~ forms
;
_journal_issue                   1
_journal_name_full               'Powder Diffraction'
_journal_page_first              33
_journal_page_last               41
_journal_paper_doi               10.1017/S0885715613001334
_journal_volume                  29
_journal_year                    2014
_chemical_formula_moiety         'F5 Fe, 2(K)'
_chemical_formula_sum            'F5 Fe K2'
_chemical_formula_weight         229.05
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   7.3964(2)
_cell_length_b                   5.6779(1)
_cell_length_c                   11.5445(3)
_cell_measurement_temperature    296
_cell_volume                     484.82(2)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      296
_diffrn_measurement_device_type  'Siemens D500'
_diffrn_measurement_method       'step scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.5418
_exptl_crystal_density_diffrn    3.138
_exptl_crystal_F_000             436.0
_pd_char_colour                  white
_pd_meas_2theta_range_inc        0.020000
_pd_meas_2theta_range_max        130.00000
_pd_meas_2theta_range_min        10.00000
_pd_meas_number_of_points        6001
_pd_proc_2theta_range_inc        0.020000
_pd_proc_2theta_range_max        129.8764
_pd_proc_2theta_range_min        9.8764
_pd_proc_ls_prof_R_factor        8.0616
_pd_proc_ls_prof_wR_expected     5.9493
_pd_proc_ls_prof_wR_factor       10.4386
_pd_proc_wavelength              1.540560
_refine_ls_goodness_of_fit_all   1.755
_refine_ls_number_parameters     70
_refine_ls_number_reflns         972
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            4.6781
_cod_data_source_file            K2FeF5-form-III.cif
_cod_data_source_block           K2FeF5-form-III
_cod_database_code               1513881
_pd_proc_ls_prof_cr_factor       13.2279
_pd_proc_ls_prof_cwr_factor      15.3081
_pd_proc_ls_prof_cwr_expected    8.7246
_pd_proc_ls_prof_chi2            3.0786
_pd_proc_ls_prof_echi2           3.0948
On two new K~2~FeF~5~ forms
Le Bail, Armel; Powder Diffraction 29 (2014) 33–41; doi:10.1017/S0885715613001334

data_1513882
_publ_contact_author_address
; 
Universit\'e du Maine, Institut des Mol\'ecules et des Mat\'eriaux du Mans, 
CNRS UMR 6283, 72085 Le Mans, France
;
_publ_contact_author_email       armel.le_bail@univ-lemans.fr
_publ_contact_author_fax         '33 (0)2 43 83 35 06'
_publ_contact_author_name        'Armel Le Bail'
_publ_contact_author_phone       '33 (0)2 43 83 33 47'
_publ_section_title
;
 On two new K~2~FeF~5~ forms
;
_journal_issue                   1
_journal_name_full               'Powder Diffraction'
_journal_page_first              33
_journal_page_last               41
_journal_paper_doi               10.1017/S0885715613001334
_journal_volume                  29
_journal_year                    2014
_chemical_formula_moiety         'F5 Fe, 2(K)'
_chemical_formula_sum            'F5 Fe K2'
_chemical_formula_weight         229.05
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90.00000
_cell_angle_beta                 118.241(1)
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   13.0919(2)
_cell_length_b                   5.7311(1)
_cell_length_c                   7.3114(1)
_cell_measurement_temperature    296
_cell_volume                     483.281(14)
_computing_structure_refinement  FULLPROF
_computing_structure_solution    ESPOIR
_diffrn_ambient_temperature      296
_diffrn_measurement_device_type  'Siemens D500'
_diffrn_measurement_method       'step scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.5418
_exptl_crystal_density_diffrn    3.148
_exptl_crystal_F_000             436.0
_pd_char_colour                  white
_pd_meas_2theta_range_inc        0.020000
_pd_meas_2theta_range_max        130.00000
_pd_meas_2theta_range_min        10.00000
_pd_meas_number_of_points        6001
_pd_proc_2theta_range_inc        0.020000
_pd_proc_2theta_range_max        129.8888
_pd_proc_2theta_range_min        9.8888
_pd_proc_ls_prof_R_factor        8.8137
_pd_proc_ls_prof_wR_expected     6.3929
_pd_proc_ls_prof_wR_factor       11.9213
_pd_proc_wavelength              1.540560
_refine_ls_goodness_of_fit_all   1.865
_refine_ls_number_parameters     55
_refine_ls_number_reflns         972
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            5.7800
_cod_data_source_file            K2FeF5-form-IV.cif
_cod_data_source_block           K2FeF5-form-IV
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               1513882
_pd_proc_ls_prof_cr_factor       14.3083
_pd_proc_ls_prof_cwr_factor      17.0215
_pd_proc_ls_prof_cwr_expected    9.1279
_pd_proc_ls_prof_chi2            3.4774
_pd_proc_ls_prof_echi2           3.5401